Download presentation

Presentation is loading. Please wait.

Published byFrancis Hefferman Modified about 1 year ago

1
The Elastic Stress Field Approach The Stress Intensity Factor The three basic modes of crack surface displacements

2
Derivation of the Elastic Stress Field Equations - Concepts of plane stress and plane strain - Equilibrium equations - Compatibility equations for strains - Airy stress function - Biharmonic equation - Complex stress functions: Westergaard function for biaxially loaded plate (Mode I) - Mode I stress / displacement fields - Mode I stress intensity factor Westergard (1939), Irwin (1957)

3
Linear Elastic Crack-tip Fields (general case) Mode I:

4
Mode III: Mode II:

5
Angular distributions of crack-tip stresses for the three modes (rectangular: left; polar:right) -Details of the applied loading enters only through K !!! for the infinite plate: K = ( *a) 1/2 - But for a given Mode there is a characteristic shape of the field !!! - Principle of Superposition: for a given Mode, K terms from superposed loadings are additive - The stress and displacement formulas may reduced to particularly simple forms: CHARACTERISTICS OF THE STRESS FIELDS

6
We consider next some other cases apart from the cracked infinite plate - Semi infinite edge notched specimens - Finite width centre cracked specimens - Finite width edge notched specimens -Crack-line loading -Elliptical / Semielliptical cracks edge notchedfinite width

7
Finite-width centre-craked specimens: Irwin: Isida: 36 term power series approx. Brown: Feddersen: f(a/W)

8
Single edge notched (SEN) Double edge notched (DEN) Finite-width edge-notched specimens: SEN: DEN: 0.5% accurate for any a/W 0.5% accurate for a/W < 0.6 Semi infinite edge- notched specimens: Free edges: crack opens more than in the infinite plate resulting in 12% increase in stress

9
TWO IMPORTANT SOLUTIONS FOR PRACTICAL USE * Crack-line Loading ( P: force per unit thickness) for centrally located force: K I decrease when crack length increases ! Crack under internal pressure ( force per unit thickness is now P.dx, where P is the internal pressure) same result by end loading with Very useful solution: - Riveted, bolted plates - Internal Pressure problems

10
* Elliptical Cracks actual cracks often initiate at surface discontinuities or corners in structural components !!! Example: corner crack in a longitudinal section of a pipe-vessel intersection in a pressure vessel We start considering idealised situations: from embeded elliptical crack to semielliptical surface cracks

11
Irwin solution for Mode I: a/c0.00.10.20.30.40.50.60.70.80.91.0 1.0001.0161.0511.0971.1511.2111.2771.3451.4181.4931.571 circular crack: The embeded (infinite plate) elliptical crack under Mode I loading Where : elliptic integral of the second type with: K I varies along the elliptical crack front max. at = /2: min. at = : During crack growth an elliptical crack will tend to become circular: important in fatigue problems

12
In practice elliptical cracks will generally occur as semi-elliptical surface cracks or quarter- elliptical corner cracks Best solutions for semielliptical: FEM calculations from Raju-Newman: Raju I.S.,Newman J.C. Jr. Stress Intensity Factors for Two Symmetric Corner Cracks, Fracture Mechanics, ASTM STP 677, pp. 411-430 (1979). The semi- elliptical surface crack in a plate of finite dimensions under Mode I loading

13
SUPERPOSITION OF STRESS INTENSITY FACTORS 1) Crack under Internal Pressure: 2) Semi-elliptical Surface Crack in a Cylindrical Pressure Vessel:

14
3) Cracks growing from both sidesof a loaded hole where the hole is small with respect to the crack where P is the force per unit thickness

15
CRACK TIP PLASTICITY First approximation:Better approaches -selected shape: better size estimation -Irwin -Dudgale -Better shape but first order approximation for the size Irwin approach: - stress redistribution; elastic – plastic; plane stress

16
First Order Aproximations of Plastic Zone Shapes Plastic zone shape from Von Mises yield criterion Through-thickness plastic zone in a plate of intermediate thickness Empirical Rules to estimating Plane Stress vs. Plane Strain conditions: -Plane Stress: 2.ry ≈ B -Plane Strain: 2.ry < 1/10 B

17
Planes of maximum shear stress: location of the planes of maximum shear stress at the tip of the crack for plane stress (a) and plane strain (b) conditions

18
Deformation Modes: plane strain (a) and plane stress (b)

19
FRACTURE TOUGHNESS Is K a useful parameter to characterise fracture toughness? Variation in K C with specimen thickness in a high strength maraging steel Under conditions of: - small scale plasticity - plane strain Kc = K IC K IC is a material property: fracture toughness of linear elastic materials

20
Effect of Specimen Thickness on Mode I Fracture Toughness Remember: Empirical Rules to estimate Plane Strain conditions: 2*ry < 1/10 B Limits to the Validity of LEFM: After considerable experimental work the following minimum specimen size requirements were established to be in a condition of : - plane strain - small scale plasticity

21
LEFM Testing: ASTM E-399, committee E8 Fatigue and Fracture Fatigue pre-cracked specimens ! ASTM Standard Single Edge notched Bend (SENB) Specimen ASTM Standard Compact Tension (CT) Specimen where

22
Clip gauge and ist attachment to the specimen Principal types of load-displacement plots obtained during KIC testing ANALYSIS -Line at 5% offset (95 % of tg OA equivalent to 2 % crack extension - Ps: intersection 5 % offset with P-v record - if there is a P value > Ps before Ps, then P Q = Ps - check if Pmax / P Q < 1.10, then - go to K(P Q ): calculate K Q (conditional K IC ) - check if for K Q the specimen size requirements are satisfied, then - check if crack front is symmetric, then K Q = K IC (valid test)

23
To provide a common scheme for describing material anisotropy, ASTM standardized the following six orientations: L-S, L-T, S-L, S-T, T-L, and T-S. The first letter denotes the direction of the applied load; the second letter denotes the direction of crack growth. In designing for fracture toughness, consideration of anisotropy is very important, as different orientations can result in widely differing fracture-toughness values. Material Toughness Anisotropy When the crack plane is parallel to the rolling direction, segregated impurities and intermetallics that lie in these planes represent easy fracture paths, and the toughness is low. When the crack plane is perpendicular to these weak planes, decohesion and crack tip blunting or stress reduction occur, effectively toughening the material. On the other hand, when the crack plane is parallel to the plane of these defects, toughness is reduced because the crack can propagate very easily.

24
Applications of Fracture Mechanics to Crack Growth at Notches S S l l 2c 2a Example: 2c = 5 mm, L* = 0.25 mm 2c = 25 mm, L* = 1.21 mm L* : transitional crack length For crack length l ≥ 10% c: crack effective length is from tip to tip!!! (including notch) Numerical Solution: Newman 1971

25
Consequences: For relatively small (5-10 % notch size) cracks at a hole or at a notch, the stress intensity factor K is approximately the same as for a much larger crack with a length that includes the hole diameter / notch depth. plane window Reading: Fatige and the Comet Airplane (taken from S. Suresh, Fatigue of Materials) Edge crack at window Crack in groove of a pressurized cylinder Lager effective crack length by a contribution of a notch !

26
SUBCRITICAL CRACK PROPAGATION IN COMPONENTS WITH PREXISTING FLAWS Fatigue Sustained load crack growth behaviour - stress corrosion cracking - cracking due to embrittlement by internal or external gaseous hydrogen - liquid metal embrittlement - creep and creep crack growth *

27
Fatigue Crack Propagation K max = K IC (1-R) !! Fatigue crack growth rate curve da/dN - K

28
How to describe crack growth rate curves: crack growth “laws“ Paris Law:only Region II, no R effects Forman: also Region III complete crack growth rate curve n1, n2, n3, empirically adjusted parameters Complete curve McEvily: the three regions

29
Fatigue crack growth rate for Structural steel (BS4360) at room temperature and with cycling frequencies 1-10 Hz. Fatigue crack growth rate vs. K for various structural materials at low R values EXAMPLES of Crack Growth rate Behaviour

30
Influence of R on fatigue crack growth in Al 2024-T3 Alclad sheet Effect of R: CRACK CLOSURE

31
Crack closure effects Measuring the crack opening stress by means of a stress-displacement curve Elber: Actually:

32
Elber obtained the empirical relationship Schijve:

33
Closure Mechanisms

34
Sustained load crack growth behaviour Time to Failure Tests: Initial K I !!! preferred technique in the past

35
Generalised sustained load crack growth behaviour K ISCC K IC or K Q Modern techniques: based on fracture mechanics parameter K !

36
SPECIMENS Increasing or decreasing K specimens crack- line wedge-loaded specimen (CLWL) bolt loaded cantilever beam- specimen (DCB) tapered double cantilever beam- specimen (TDCB): constant K !!!

37
Difference in crack growth behaviour for increasing K (cantilever beam) and decreasing K (modified CLWL or DCB specimens) Decreasing K specimens: Advantages: Disadvantages: Entire crack growth with one specimen Self stressed and portable Clear steady state and arrest Corrosion product wedging: gives higher crack growth rate at a given nominal KI.

38
Example: Outdoor exposure stress corrosion cracking propagation in 7000 series Al-alloy plate

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google